Upcoming SlideShare
×

# 7.metal forming bending 1

1,046 views
885 views

Published on

0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total views
1,046
On SlideShare
0
From Embeds
0
Number of Embeds
4
Actions
Shares
0
55
0
Likes
0
Embeds 0
No embeds

No notes for slide

### 7.metal forming bending 1

1. 1. IE 337: Materials and Manufacturing Processes Lab # 7 Metal Forming: BendingIntroduction: Sheet metal working generally incorporates cutting and forming operations on thin sheets ofmetal. Typically, the thickness of sheet metal is between ¼ inch and 1/64 inch. There are differenttypes of metal forming operations: Bending, Shearing, Blanking, Punching, Stamping etc. This labprovides an exposure to BENDING operation. Bending is defined as the straining of the metal around a straight axis (Figure 7.1). During thebending process, the metal on the inside of the neutral plane is compressed, while the metal on theoutside is stretched. The sheet metal is plastically deformed to have a permanent bent shape. Bendingproduces a little or no thickness change of the sheet metal.Figure 7.1. (a) Sheet metal bending, and (b) compression and tensile elongation during bending. In the Figure 7.1, α = bend angle, w = width of sheet, R = bend radius, t = sheet thickness, andα′ = 180° - α, “included” angle. In this lab we will work on V-bending. Typically, a bendingoperation is performed using a punch and die. In V-bending the sheet metal is bent between a V-shaped punch and die. The operation is shown in Figure 7.2. When the bending stress is removed atthe end of the deformation process, elastic energy remains in the bent part causing it to partiallyrecover to its original shape. In bending, this elastic recovery is called springback (SB). It increaseswith decreasing the modulus of elasticity, E, and increasing the yield strength, Y, of a material.Springback is defined as the increase in included angle of the bent part relative to the included angleof the forming tool after the tool is removed. After springback, the bend angle will decrease (theincluded angle will increase) and the bend radius will increase. D Figure 7.2. V-bending operation. 1 March 3, 2010
2. 2. IE 337: Materials and Manufacturing Processes Lab # 7 Metal Forming: Bending ………………………….. 7.1where, α’ is included angle of the sheet-metal part (bend angle) in degrees and α’t is the includedangle of the bending tool (Die angle) in degrees. Bending force can be calculated with help ofequation 7.2. ……………………….... 7.2where, F is bending force (lb), TS is tensile strength of the sheet metal (lb/in2), w is width of the partin the direction of the bend axis (in), t is the sheet-metal thickness (in), and D is the die openingdimension (in). Kbf is a constant that accounts for differences encountered in actual bending processand is 1.33 for V-bending.Objective: 1. To understand the basic bending operation 2. To study the effects of material properties (ductility, types, strength) on the bend radius, springback and bending forceEquipment: 1. Tooling dies with 0 bend radius, (1.5*thickness) bend radius and (3*thickness) bend radius 2. Arbor press 3. Work pieces a. Half Hardened C26000 brass: 1/8” and 1/16” thicknesses b. Precipitation hardened 6061 Al alloy: 1/8” and 1/16” thicknesses c. Mild Steel 1018 1/8” and 1/16” thicknesses 4. Protractor 5. Calipers/MicrometerProcedure: 1. Insert the 0 bend radius die into the arbor press. 2. Insert the work piece into the holder. 3. Pull down the handle on the press firmly. 4. Check for material failure (cracking at the bend). Measure the bend radius. Record results on data sheet provided. 5. Repeat steps 1-4 for each type of material. 6. Repeat steps 1-5 for each bend radiusLab Deliverables: 1. Prepare a report detailing the lab activity, observations, results and difficulties faced (follow the lab report instructions). 2. Plot the following function for the different materials (R vs t) 2 March 3, 2010
3. 3. IE 337: Materials and Manufacturing Processes Lab # 7 Metal Forming: Bending 1 % R = Minimum bend radius t = Material thickness %A = Tensile reduction in area %E= % of elongation at break % % 100 % The area of the graph above and to the left of this line is supposed to result in ductile bending without failure. The area below and to the right represents processing conditions that will result in material cracking. Plot the experimental values used in lab on this graph. Do these values make sense? What is the effect of ductility on minimum bend radius?(5) 3. What is the effect of ductility on spring back? Is there a consistent trend? Does this relationship make sense? Which material would permit better bend tolerances?(4) 4. Calculate the bending force for each case. Compare the bending forces required for hardened brass vs. annealed brass for different thicknesses and die opening.(6) 5. Tabulate the springback vs. thickness for the different materials and explain the trend based on their young’s modulus.(5)Appendix:Table 1: Elastic properties of the given materials Young’s Poisson’s % Elongation at Ys Material modulus TS (MPa) ratio break (MPa) (GPa) 425 (half hardened) C26000 0.375 110 23 525 (hardened) 360 Brass 325 (annealed) Al 6061 0.330 69 12 310 276 Alloy 1018 Steel 0.290 205 15 440 370Section wise maximum marks: Intro – 10, Objectives – 5, Procedure – 15, Results and discussion –15, conclusion – 10, Deliverables - 20 3 March 3, 2010
4. 4. IE 337: Materials and Manufacturing Processes Lab # 7 Metal Forming: BendingReferences: 1. M.P. Groover, “Fundamentals of modern manufacturing,” 3rd edition, (2007). 2. S. Kalpukjian, S.R. Schmid, “Manufacturing procedure for engineering materials,” 2nd edition, p. 350-351. 4 March 3, 2010